reproducibility of critical chloride threshold levels for
REPRODUCIBILITY OF CRITICAL CHLORIDE THRESHOLD LEVELS FOR
STAINLESS STEEL REINFORCEMENT
S. Randström, M. Almén, R. Pettersson
Outokumpu Stainless AB
Avesta Research Centre
SE-774 22 Avesta
Outokumpu Stainless Ltd.
ASR Rod Mill
Sheffield S9 3XG
KEY-WORDS: Stainless steel reinforcement, Critical Chloride Threshold Level, Chlorides
Corrosion resistant reinforcement is crucial in order to reduce the repair cost of corroding concrete
structures. In the hunt for lower cost and high performance reinforcement, a measure of the chloride
tolerance is needed to select the proper material based on the surface chloride content, the concrete type
and the surrounding temperature. Critical Chloride Threshold Level (CCTL) measurements have been
performed over the past 40 years to investigate the chloride tolerance of different reinforcement materials,
but a standardized method that gives a fast and reliable response still does not exist. In this article, a
potentiostatic in-solution method, which has been used by other researchers, is used for determining the
CCTL of different stainless steel grades. The reproducibility of the method and the influence of the
condition of the stainless steel reinforcement on the CCTL are investigated. The results indicate that there
is some scatter in the results also for stainless steels and it is better to define the CCTL as a probability
distribution based on a number of replicates for each stainless steel grade instead of a discrete number.
Stainless steel reinforcement is a maintenance-free solution for corroding concrete structures due to the
superior corrosion resistance of stainless steels compared to carbon steels or other metallic reinforcing
bars. The stainless steel reinforcement is used selectively, with only the outermost layers of the carbon
steel reinforcement replaced with the more corrosion-resistant reinforcement. This makes the investment
attractive, with only a minor increase in the initial cost, and a much lower maintenance cost during the
Determination of the corrosion resistance of steels in concrete is very different to corrosion testing for
many other applications. The diffusion rate of chlorides is comparatively slow, the presence of the
sponge-like concrete affects transport rates of both gases and liquids and the alkaline environment
increases the chloride tolerance, so long as the pH does not drop due to carbonation. As a result,
accelerated testing is needed, where some parameters are assumed to either a) not affect the corrosion
resistance or b) affect the corrosion resistance to a controlled degree.
Over the years, the corrosion resistance of the stainless steels rebars has been determined by many
different methods. Mainly two different ways to determine the corrosion resistance have been used, castin testing and testing in the concrete pore-solution. An extended discussion of these methods can be found
in an earlier paper (Randström and Adair 2009). Cast-in testing, which resembles the real application
most, can be advantageous since the method enables that chlorides slowly diffuse into the concrete
structure, as they do in a real structure. However, using this method, the testing times are often some
years or even longer, and the exact chloride level at the position where the corrosion started can
sometimes be difficult to determine. The onset of corrosion on stainless steels can also be difficult to
detect when the rebar is cast-in (Hurley and Scully, 2006). Frequently, the use of Linear Polarisation
Resistance (LPR) is used to determine whether the stainless steel is active or still passive. This method,
requires a significant part of the material to be active, and is therefore better to use on low-alloyed steel
where chlorides cause activation of a larger surface than on stainless steel rebars, where chlorides cause
localized corrosion. In addition, the corrosion potential is often measured to determine whether corrosion
has occurred. The corrosion potential measurement is an easy, non-destructive method to detect possible
corrosion in structures and bridges made of carbon steel. According to the standard ASTM C876,which is
a standard for half-cell potential measurements of reinforcement in concrete, the probability that the
carbon steel reinforcement is corroding if the potential is below -280 mVSCE (mV versus the standard
calomel electrode) is over 90%. However, if the oxygen level is low, the above mentioned potential can
be measured without any corrosion occurring. For laboratory-experiments, where shorter times are
investigated, the oxygen level can be low due to completely water-filled pores, so it is strongly
recommended that corrosion is confirmed by visual inspection and/or weight loss measurements. For
stainless steels a recent report (Sederholm and Almqvist, 2008) showed that cast-in stainless steels can
have potentials more negative than -280 mVSCE for several months without showing any signs of
corrosion by visual inspection and weight loss measurements.
For the purpose of determining chloride levels and for ranking corrosion resistance, a potentiostatic test in
synthetic pore-solution can be more useful. In this case, a solution similar to that found in the pores of the
concrete is used. The composition of such pore-solutions is mainly based on hydroxides of sodium,
potassium and calcium (Bertolini et al., 2004). Although these tests do not take the solid concrete matrix
into account, they can predict the corrosion resistance and the chloride tolerance in this alkaline
environment in a fast and efficient way. A potentiostatic method has proved useful to determine the
chloride tolerance since onset of the local corrosion attack is immediately detected by the increase in
current (Bertolini et al., 1996), (Hurley and Scully, 2006). In this method, the rebar specimen is polarized
to a fixed potential (often +200 mVSCE) in a chloride-free synthetic pore-solution. The chlorides are
thereafter added incrementally until corrosion occurs. A corrosion test using this method takes around two
weeks to perform and different solutions can be used.
Stainless steel rebars with diameters ranging from 8-25 mm were used in four different stainless steel
grades, with both austenitic and duplex microstructures. The nominal compositions of these grades are
seen in Table 1 and the rebars were all commercially produced by Outokumpu. The rebars were cut in
10 cm lengths and a hole (4 mm) for electrical contact was drilled in one of the ends of the rebar. For
investigation of the surface effect, some of the rebars were first sand-blasted with aluminium silicate. All
rebars were thereafter ultrasonically cleaned in acetone for 20 min, and covered with Lacomit (Agar
Scientific) in both ends.
Table 1 Nominal composition of the stainless steel grades used
The prepared rebars were hung in a QuickFit beaker and a ring counter-electrode of platinum was placed
around it. A Luggin capillary was placed close to the hanging rebar and connected to a standard calomel
electrode (SCE). All potentials will hereafter be referred to this reference electrode. 1 L of pore solution,
with a composition of 2.61 g/L NaOH, 9.04 g/L KOH and 0.17 g/L Ca(OH)2 (hereafter referred to as
OPC solution) was poured into the beaker. The rebar was adjusted so that the water line was at the
Lacomit-covered area. Air, scrubbed through a wash bottle containing 3g/L Ca(OH)2 in water was
bubbled through the solution to promote stirring and saturate the electrolyte with oxygen. The setup is
seen in Figure 1.
Figure 1Schematic view of the cell setup
The open circuit potential (OCP) was measured for 1.5 h before the experiment started (OCP part), and
the potential was thereafter increased from 25 mV below the open circuit potential to the final
potential,+200 mVSCE with a scan rate of 10 mV·min-1 (Linear Polarisation part). The potential was
thereafter held at this potential throughout the experiment (Chronoamperometric part). Chlorides were
added after at least 10 h had passed at this potential. This potential has been selected by other research
groups and is believed to give conservative results. It corresponds to an overpotential of more than
400 mV, since open circuit potentials in this alkaline environment normally are around -200 mVSCE
(Hurley and Scully, 2006).
Chloride additions were made by replacing a certain amount of the synthetic pore solution with a solution
of the same composition but with a sodium chloride concentration of 5 M. These additions were made
every 12th hour. The volume replaced was selected so that the chloride concentration in the electrolyte
was increased by 0.1 M every chloride addition.
The CCTL was defined as the chloride content at which the current density exceeded 10 µA·cm-2 for 5 h.
When CCTL was reached, a sample of the electrolyte was transferred to an air-tight bottle to measure pH
and chlorides. pH was measured after the experiment with a pH meter (Jenway 3345 Ion meter equipped
with a Schott pH electrode - Blue line) or a combined pH /chloride measurement unit (Mettler Toledo
SevenMulti S80 equipped with an InLab Routine Pro pH-electrode and a DX235-Cl/InLab Reference
electrode for chloride measurements).
RESULTS AND DISCUSSION
An example of the OCP and chronoamperometric part of the electrochemical experiment is seen in Figure
2. The increase in current density in this case started within 2 hours after the last addition of chlorides,
resulting in a chloride concentration of 6.4 wt% which was determined as the CCTL. The very long
incubation time of the corrosion supports the theory that polarization curves may be a too fast method to
determine CCTL, a discussion earlier brought up by (Hurley and Scully, 2006). In their study, the CCTL
determined by a potentiodynamic method was higher compared to when a potentiostatic method with
incremental chloride additions was used. It is therefore important to note what kind of method that has
been used to determine the CCTL when data is compared.
Figure 2 Left: Open circuit potential (corrosion potential) of a rebar specimen in this experiment. Right: Example of
curve during the chronoamperometric part of the experiment, from the first chloride addition. The graph illustrates a
316 rebar specimen. The time which chloride additions were made are marked with red diamond markers.
In the test, the corrosion at the stainless steel rebar typically starts as a spot where corrosion products are
deposited, as seen in Figure 3. The corrosion propagates and a larger area is covered with corrosion
products, as seen in the right part of Figure 3. The propagation is sometimes very slow, and the corrosion
at the spot can stop so the current decreases to a low value. Therefore, the CCTL was defined as the
chloride concentration where propagating corrosion occurred.
Figure 3 The onset of corrosion attack on a stainless steel rebar when using the potentiostatic method. The right image
is taken approximately 30 minutes after the left image. Note that a high potential was applied to the specimen, forcing
the corrosion to occur rapidly
The CCTL values determined by this potentiostatic method for the four different grades are seen in Figure
4. The figure shows test results from commercially produced rebars, and the corrosion resistance shown is
therefore representative for stainless steel rebars that are delivered to the customer.
Figure 4 CCTL values of the different stainless steel grades
The results indicate that there is no significant difference in corrosion resistance between 316L, LDX
2101® and 2304, while 304L has a slightly lower CCTL. The results correspond fairly well with those
from other researchers who have used a similar potentiostatic method, as can be seen in Table 2. The
largest deviation compared to other authors is seen for LDX 2101®, which clearly has a corrosion
resistance comparable to 316L in this study, but was reported to have a corrosion resistance lower than
316L in the study by (Hurley and Scully, 2006) and (Bertolini et al., 2009). In the case of (Hurley and
Scully, 2006), the LDX 2101® it was stated that the rebar was laboratory pickled, which could be the
reason for the difference in corrosion resistance.
Table 2 CCTL values in wt% chlorides for the investigated stainless steel rebar grades. Comparisons with other groups
using a similar method have also been added, with additional data of low-chromium alloys not included in this study.
Numbers in brackets represent the numbers of rebar tested.
pH (after test)
LDX 2101® -type
Bertolini et al.
[No. of specimens
tested not stated]
Bertolini et al.
Hurley and Scully
6.5-10 (304LN) 
>10 (316LN) 
2.8-11.29 (316LN) 
The pickling time has an effect on the corrosion resistance in potentiostatic tests. The chloride tolerance
of three different surface types for LDX 2101®, seen in Figure 5 was investigated and the result can be
seen in Figure 6. The over-pickled surface, shown in the left image in Figure 5, had many micro-crevices
in the outermost layers of the stainless steel rebar and clearly has a lower corrosion resistance compared
to normally pickled LDX 2101®. These types of micro-crevices are typical when stainless steels are overpickled particularly if they contain precipitates which increase the pickling rate at the grain boundaries.
Grain boundary precipitates are introduced by faulty heat-treatments or when carbon contents are too
high. This could explain the low corrosion resistance of the 2101-type stainless rebar tested by (Bertolini
et al. 2009), since the carbon content was 0.049, well above the normal carbon content for LDX 2101®. It
can therefore be stated that the pickling procedure and melt composition is critical in order to obtain
satisfactory performance of the material. It is moreover important to consider the surface condition when
rebars in different grades are compared, and it is vital for a producer to deliver material with good
surfaces with optimal corrosion resistance.
A sand-blasted surface, included in Figure 5 and Figure 6, was found to have the same CCTL as a
normally pickled surface. If such an operation is used, it should be verified that the surface after treatment
is reasonably smooth without embedded particles. As with all sand-blasting of stainless steels, it is also
critical to ensure that the blasting sand has not been contaminated by previous use on carbon steel. Such
contaminated sand can very quickly lead to rust speckling on the stainless steel because of embedded
carbon steel particles.
Figure 5 Surface of over-pickled (left), normally pickled (middle) and sand-blasted rebar (right).
Figure 6 Effect of surface modification (over-pickling and sand-blasting) of LDX 2101
The scatter seen in the results in Figure 4 as well as in the study of (Hurley and Scully, 2006), brings up
the discussion whether it is correct to define the CCTL value as a discrete number or if it is better to
define it as a probability that the stainless steel rebar corrodes. If it is assumed that the data values are
normally distributed, a probability plot, can be made as shown in Figure 7. This plot emphasizes a
number of the points made qualitatively earlier in the paper. Firstly it is seen that at the 90% probability
level, indicated with a grey circle, there is good correspondence between the CCTL levels for 316L, LDX
2101® and 2304, while that for 304L is significantly lower. Secondly the slope of the curves, which is
related to the standard deviation in the measurements, is similar for 304L, LDX 2101® and 2304, but
somewhat lower for 316L. This type of plot is very common for e.g. life-time predictions and is strongly
recommended as an assessment tool for CCTL data because of the scatter seen in the measurements.
Figure 7 Probability graph assuming that the CCTL results are normally distributed
A chloride threshold based on the concept of a statistical distribution has earlier been introduced for
carbon steels cast in concrete (Glass 1995), (Browne 1982), and mentioned in Concrete Society’s
Technical Report 61 (Bamforth, 2004) suggesting that corrosion of carbon steel should be considered as
an increased probability for corrosion rather than a discrete value. The probability classification proposed
by (Browne 1982) is shown in Table 3.
Table 3 Probability classification of carbon steel rebar seen in Concrete Society Technical Report 61 (Bamforth 2004),
proposed by (Browne 1982)
Chloride (% weight of cement)
Risk of corrosion
The threshold limit for carbon steel differs between regions. In the USA, the value of 0.2% chlorides per
mass of cement is often regarded as the limit, while 0.4% is often mentioned as the limit in Europe. This
seems to correspond to a probability that the reinforcement is not corroding of 90% and 80%, respectively
(Bamforth, 2004). Using these probability percentage for the stainless steel reinforcement investigated in
this study, especially for LDX 2101®, that has been tested nine times; the difference in CCTL using these
to criteria would be around 1wt%. Although the difference is not very large, it is recommended that a
90% probability criterion is used, since this is a more conservative result, and since it underlines the need
for a large number of tests to determine eventual differences between stainless steel grades.
Compared to cast-in rebars, the environment (pH, temperature, conductivity, chloride and oxygen levels)
is more strictly controlled in the pore-solution test. The scatter of the results therefore indicates that it is
related to the variability in corrosion initiation and propagation processes. Such variability could explain
the scatter of data both seen in cast-in experiments (Alonso et al, 2006) and other pore-solution tests
(Hurley and Scully, 2006) when a significant number of specimen have been investigated.
The potentiostatic method used in this article differs from the real situation in the concrete structure
regarding transport rates of oxygen and chlorides but nevertheless gives an idea what to expect in terms of
corrosion resistance. The applied potential of +200 mVSCE in the potentiostatic tests corresponds to a
large overpotential of around 400 mV, which is believed to give conservative results. On the other hand,
the solid concrete matrix in cast-in tests creates crevices, which could decrease the corrosion resistance.
Recently, (Bertolini et al., 2009) suggested that potentiostatic tests were misleading since they lacked
correlation to cast-in tests. However, this conclusion was based on two measurements in pore-solution
and corrosion potentials plus LPR measurements of sometimes only single specimens in concrete blocks
with different chloride levels. Of course, it is difficult to predict what will happen in a real application,
and there will likely be some discrepancies between pore-solution tests, cast-in tests and the real
application, as there is for all comparisons between lab-scale testing and the industrial application.
Nevertheless, for the understanding of the chloride tolerance of stainless steel in this application it is very
important to start with a few controlled parameters and thereafter move on by adding more unknown
parameters, with control of the scatter and limitations of the method used at each step.
In this study, stainless steel rebars in four different grades have been tested. At least five different
specimens were tested for each grade, to allow assessment of the scatter of the method. The results
indicate that 316L, LDX 2101®, and 2304 have similar corrosion resistance while 304L has slightly lower
corrosion resistance. The results are generally in agreement with what other researchers have found
except for the fact that this study shows that LDX 2101® has similar corrosion resistance to 316L. It has
also been demonstrated that over-pickling of the LDX 2101® material decreases the corrosion resistance,
which could explain the lower corrosion resistance reported for this grade.
The scatter of the results is quite large even though the parameters are carefully controlled in this method.
There is therefore a risk that making only one or two measurements can give completely misleading
results. Even when the surface is normalized by sand-blasting, the scatter seems to remain. Therefore, it is
much more relevant to describe the chloride tolerance of stainless steel rebars as a probability distribution
rather than as a discrete, critical value. This is in line with the approach used for carbon steel that has
been cast in concrete. It would appear that the value of 0.2% chloride by mass of cement used for carbon
steel in the USA would correspond to 90% probability and the European figure of 0.4% chlorides
correspond to 80% probability. The analysis of this research would indicate that a value of 90%
probability should be used for stainless steel rebar.
Alonso C., Castellote M., Andrade C. (2002) Chloride Threshold dependence of pitting potential
of reinforcements, Electrochim. Acta, 47, 3469-3481
Bamforth P.B. (2004) Enhancing reinforced concrete durability, Concrete Society Technical
Report 61, The Concrete Society, Surrey
Bertolini L, Bolzoni F, Pastore T, Pedeferri P. (1996) Behaviour of stainless steel in simulated
concrete, Br. Corr. J. 31, 218-222.
Bertolini, L., Elsener, B., Pedeferri, P., Polder, R. (2004) Corrosion of steel in concrete WileyVCH, Weinheim
Bertolini L., Gastaldi M. Corrosion resistance of austenitic and low-nickel duplex stainless steel
bars, Eurocorr 2009, 6-9 September 2009, Nice
Browne R.D. (1982) Design prediction of the life of reinforced concrete in marine and other
chloride environments, Durability of Building Materials, Vol. 3, Elsevier Scientific, Amsterdam
Glass GK (1995) The determination of chloride binding relationships, International RILEM
Workshop on Chloride penetration into concrete St-Remy-Les-Chevreuse, October 15-18 1995
Eds. Nilsson L.O. and Olivier, J.P.
Hurley MF, Scully JR (2006) Threshold Chloride Concentrations of Selected Corrosion-Resistant
Rebar Materials Compared to Carbon Steel, Corr. Sci. 62, 892-904.
Randström S., Adair M. (2009) Critical Chloride threshold levels for stainless steel reinforcement
in pore solutions, Paper no. 046, Corrosion and Prevention 2009, Coffs Harbour, 15-19 November
Sederholm, B., Almqvist, J. (2008) Stainless steel in concrete – Galvanic effects on carbon steel,
Report no. KIMAB 2008-133, Swerea KIMAB, Stockholm